#------------------------------------------------------------------------------
#$Date: 2024-05-16 08:36:09 +0200 (Thu 16 de May de 2024) $
#$Revision: 291877 $
#$URL: svn://www.crystallography.net/cod/cif/9/01/18/9011817.cif $
#------------------------------------------------------------------------------
#
# This file is available in the Crystallography Open Database (COD),
# http://www.crystallography.net/. The original data for this entry
# were provided the American Mineralogist Crystal Structure Database,
# http://rruff.geo.arizona.edu/AMS/amcsd.php
#
# The file may be used within the scientific community so long as
# proper attribution is given to the journal article from which the
# data were obtained.
#
data_9011817
loop_
_publ_author_name
'Kyono, A.'
'Kimata, M.'
_publ_section_title
;
 Refinement of the crystal structure of a synthetic non-stoichiometric
 Rb-feldspar
;
_journal_issue                   4
_journal_name_full               'Mineralogical Magazine'
_journal_page_first              523
_journal_page_last               531
_journal_paper_doi               10.1180/002646101750377542
_journal_volume                  65
_journal_year                    2001
_chemical_compound_source        Synthetic
_chemical_formula_sum            'Al1.062 O8 Rb0.811 Si3'
_chemical_name_mineral           Rubicline
_space_group_IT_number           12
_symmetry_space_group_name_Hall  '-C 2y'
_symmetry_space_group_name_H-M   'C 1 2/m 1'
_cell_angle_alpha                90
_cell_angle_beta                 116.11
_cell_angle_gamma                90
_cell_length_a                   8.839
_cell_length_b                   13.035
_cell_length_c                   7.175
_cell_formula_units_Z            4
_cell_volume                     742.316
_database_code_amcsd             0014559
_exptl_crystal_density_diffrn    2.776
_cod_depositor_comments
;
 Adding _atom_site_type_symbol label and values.

 Antanas Vaitkus
 2013-03-28
;
_cod_original_formula_sum        'Rb.811 Al1.062 Si3 O8'
_cod_database_code               9011817
loop_
_space_group_symop_operation_xyz
x,y,z
1/2+x,1/2+y,z
x,-y,z
1/2+x,1/2-y,z
-x,y,-z
1/2-x,1/2+y,-z
-x,-y,-z
1/2-x,1/2-y,-z
loop_
_atom_site_label
_atom_site_type_symbol
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_occupancy
_atom_site_U_iso_or_equiv
Rb Rb 0.29600 0.00000 0.14600 0.81100 0.04540
Al Al 0.29600 0.00000 0.14600 0.06200 0.04540
SiT1 Si 0.01060 0.19130 0.22230 0.75500 0.04740
AlT2 Al 0.01060 0.19130 0.22230 0.24500 0.04740
SiT2 Si 0.72350 0.11940 0.34460 0.74500 0.04920
AlT2 Al 0.72350 0.11940 0.34460 0.25500 0.04940
OA1 O 0.00000 0.15570 0.00000 1.00000 0.06300
OA2 O 0.66620 0.00000 0.28340 1.00000 0.04900
OB O 0.83110 0.15970 0.22450 1.00000 0.06450
OC O 0.04440 0.31300 0.25850 1.00000 0.06460
OD O 0.16920 0.12920 0.40260 1.00000 0.05600
loop_
_cod_related_entry_id
_cod_related_entry_database
_cod_related_entry_code
1 AMCSD 0014559
